2 DefectA flaw or flaws that by nature or accumulated effect render a part or product unable to meet minimum applicable acceptance standards or specifications. The term designates rejectability.
3 DiscontinuityAn interruption of the typical structure of a material, such as a lack of homogeneity in its mechanical, metallurgical, or physical characteristics. A discontinuity is not necessarily a defect.
4 Weld Joint Discontinuities Misalignment (hi-lo)UndercutUnderfillConcavity or ConvexityExcessive reinforcementImproper reinforcementOverlapBurn-throughIncomplete or Insufficient PenetrationIncomplete FusionSurface irregularityArc StrikesInclusionsSlagWagontracksTungstenSpatterArc CratersCracksLongitudinalTransverseCraterThroatToeRootUnderbeadHotCold or delayedBase Metal DiscontinuitiesLamellar tearingLaminations and DelaminationsLaps and SeamsPorosityUniformly ScatteredClusterLinearPipingHeat-affected zone microstructure alterationBase Plate laminationsSize or dimensions
5 Dimensional DefectsA Dimensional defects are any defect that cause the weld metal. Parent metal, work piece to be out of specification or tolerance.Dimensional defects are mainly caused by improper set up or distortion. This should be managed before the welding process.
6 Misalignment (hi-lo)Definition: Amount a joint is out of alignment at the rootCause: Carelessness. Also due to joining different thicknesses (transition thickness)Prevention: Workmanship. Transition angles not to exceed 2.5 to 1.Repair: Grinding. Careful on surface finish and direction of grind marks. Inside of Pipe /Tube difficult.
8 UndercutDefinition: A groove cut at the toe of the weld and left unfilled.Cause: High amperage, electrode angle, long arc length, rustPrevention: Set machine on scrap metal. Clean metal before welding.Repair: Weld with smaller electrode, sometimes must be low hydrogen with preheat.
9 Undercut (cont......)Undercut typically has an allowable limit. Different codes and standards vary greatly in the allowable amount. Plate - the lesser of 1/32” or 5% (typ.)
12 Insufficient FillDefinition: The weld surface is below the adjacent surfaces of the base metalCause: Improper welding techniquesPrevention: Apply proper welding techniques for the weld type and position.Repair: Simply weld to fill. May require preparation by grinding.
14 Concave and convex weld profiles The concave defect cause the weld to be weak across the throat of the weld (Middle).The cause of this are:Travel speed is to quickAmps are to highPoor electrode Manipulation
15 Concave and convex weld profiles The convex defect cause the weld to become weak at the toes of the weld (outer edges).This is caused by :Travel speed being to slowAmps to lowPoor electrode manipulation.
16 Excessive Concavity or Convexity Definition: Concavity or convexity of a fillet weld which exceeds the specified allowable limitsCause: Amperage and travel speedPrevention: Observe proper parameters and techniques.Repair: Grind off or weld on. Must blend smoothly into the base metal.
22 ReinforcementThe amount of a groove weld which extends beyond the surface of the plateExcessiveInsufficientImproper contourFace ReinforcementRoot Reinforcement
23 Excessive Reinforcement Definition: Specifically defined by the standard. Typically, Reinforcement should be flush to 1/16”(pipe) or flush to 1/8” (plate or structural shapes).Cause: Travel speed too slow, amperage too lowPrevention: Set amperage and travel speed on scrap plate.Repair: Remove excessive reinforcement and feather the weld toes to a smooth transition to the base plate.
25 Insufficient Reinforcement Definition: Specifically defined by the standard. Typically, Underfill may be up to 5% of metal thickness not to exceed 1/32” as long as the thickness is made up in the opposite reinforcement.Prevention: Use proper welding technique. Use backing or consumable inserts. Use back weld or backing.Repair: Possibly simply increase the face reinforcement. If backwelding is not possible, must remove and reweld.
26 Improper Weld ContourDefinition: When the weld exhibits less than a 1350 transition angle at the weld toe.1350Cause: Poor welding techniquePrevention: Use proper techniques. A weave or whip motion can often eliminate the problem.Repair: The weld face must be feathered into the base plate.
28 OverlapDefinition: When the face of the weld extends beyond the toe of the weldCause: Improper welding technique. Typically, electrode angles and travel speed.Prevention: Overlap is a contour problem. Proper welding technique will prevent this problem.Repair: Overlap must be removed to blend smoothly into the base metal. Be careful of deep grind marks that run transverse to the load. Also be careful of fusion discontinuities hidden by grinding. Use NDT to be sure.
29 OverlapOverlap is measured with a square edge such as a 6” rule. No amount of overlap is typically allowed.
31 Burn-throughDefinition: When an undesirable open hole has been completely melted through the base metal. The hole may or may not be left open.Cause: Excessive heat input.Prevention: Reduce heat input by increasing travel speed, use of a heat sink, or by reducing welding parameters.Repair: Will be defined by standards. Filling may suffice. Otherwise, removal and rewelding may be required. Some standards may require special filler metal.
33 Incomplete fusion and Penetration Incomplete root fusion is when theweld fails to fuse one side of thejoint in the root. Incomplete rootpenetration occurs when bothsides of the joint are unfused.Some of the causes are:-Excessively thick root gap.Too small a root gapMisaligned weldsPower input to lowArc (heat) input to lowThese defects can be reduced in MMA welding byUsing the correct welding parameters andElectrode size, This will give the correct arc energyInput. a) b) c) d) e)
34 Incomplete or Insufficient Penetration Definition: When the weld metal does not extend to the required depth into the joint rootCause: Low amperage, low preheat, tight root opening, fast travel speed, short arc length.Prevention: Correct the contributing factor(s).Repair: Back gouge and back weld or remove and reweld.
36 Incomplete FusionDefinition: Where weld metal does not form a cohesive bond with the base metal.Cause: Low amperage, steep electrode angles, fast travel speed, short arc gap, lack of preheat, electrode too small, unclean base metal.Prevention: Eliminate the potential causes.Repair: remove and reweld, being careful to completely remove the defective area. This is sometimes extremely difficult to find.
39 Arc Strike Definition: A localized coalescence outside the weld zone. Cause: CarelessnessPrevention: In difficult areas, adjacent areas can be protected using fire blankets.Repair: Where applicable, arc strikes must be sanded smooth and tested for cracks. If found, they must be remove and repaired using a qualified repair procedure and inspected as any other weld.
42 Slag Inclusion Definition: Slag entrapped within the weld Cause: Low amperage, improper technique, Trying to weld in an area that is too tight. Slow travel in Vertical DownPrevention: Increase amperage or preheat, grind out tight areas to gain access to bottom of joint.Repair: Remove by grinding. Reweld.
44 Wagon TracksDefinition: Slang term for a groove left at the toe of a root pass which becomes filled with slag and is trapped in the weld.Cause: The contour of the root pass is too high, or the weld toe is not bonded to the base metalPrevention: Use proper technique to deposit the weld root.Repair: Carefully grind the root pass face flat. be careful not to gouge other areas on the weldment.
46 Tungsten InclusionDefinition: A tungsten particle embedded in a weld. (Typically GTAW only)Cause: Tungsten electrode too small, amperage too high, AC balance on +, Upslope too high, electrode tip not snipped, electrode dipped into the weld pool or touched with the fill rod, electrode split.Prevention: Eliminate the causeRepair: Grind out and reweld
47 SpatterDefinition: Small particles of weld metal expelled from the welding operation which adhere to the base metal surface.Cause: Long arc length, severe electrode angles, high amperages.Prevention: Correct the cause. Base metal can be protected with coverings or hi-temp paints.Repair: Remove by grinding or sanding. Sometimes must be tested as if it were a weld.